Adsorptive Removal of Fluoride onto Different Waste Materials: Orange Juice Residue, Waste Seaweed, and Spent Cation-Exchange Resin

*Katsutoshi Inoue, Hari Paudyal, Hidetaka Kawakita and Keisuke Ohto*

## **Abstract**

To effectively use waste materials in developing a sustainable society, adsorbents for removing trace or low concentrations of fluoride, which is difficult to be removed by conventional techniques, were prepared from three waste materials: orange juice residue, waste sea weed, and spent cation exchange resin. These adsorbents were loaded with tri- or tetravalent metal ions such as iron(III) and zirconium(IV), of which zirconium(IV) was found to be most suitable as the loaded metal ion. From the pH effect on adsorption, the adsorption mechanism was inferred, and adsorption and desorption was found to be controlled by changing pH values. The maximum adsorption capacities on zirconium(IV)-loaded orange juice residue, waste sea weed, and spent cation exchange resin were evaluated as 33.1, 18.1, and 37.6 mg/g, respectively, which were higher than those of most other adsorbents reported in literatures. They exhibited high selectivity for fluoride over other anionic species and high durability. Tests to remove trace concentrations of fluoride from actual waste plating solutions revealed that the concentration could be reduced below the acceptable level using small amounts of these adsorbents, i.e., it was reduced lower than 1.5 mg/dm3 (WHO standard) by adding 1 g of the adsorbents into 1 dm3 test solution.

**Keywords:** adsorptive removal of fluoride, waste materials, orange juice residue, waste seaweed, spent cation-exchange resin, zirconium(IV)-loaded adsorbents

## **1. Introduction**

Fluoride is contained in effluents from various industries, such as plating, productions of silicon semiconductors and solar panels, nuclear fuels, and phosphoric acid from phosphate rocks, as well as the refining of niobium and tantalum. The conventional technique for removing fluoride from such effluents is by precipitation as calcium fluoride by adding calcium, such as in the form of lime; however, because of the low solubility product of calcium fluoride

(Ksp = 3.9 × 10<sup>−</sup>11 (e.g., see [1])), it is theoretically difficult to lower the concentration to less than 8 mg dm<sup>−</sup><sup>3</sup> and practically difficult to achieve less than 10 mg dm<sup>−</sup><sup>3</sup> . The maximum acceptable limit of fluoride in drinking water is 1.5 mg dm<sup>−</sup><sup>3</sup> (e.g., see [2]). Consequently, some additional treatment is necessary to meet the regulation for fluoride before discharging industrial waste solutions into the environment. Adsorption techniques, including ion-exchange, are most suitable to remove such trace concentrations of contaminants in water. According to the well-known Hoffmeister's selectivity series of anion-exchange [3], the selectivity of usual anion-exchange resins for fluoride over other anionic species, such as sulfate and chloride (which usually coexist together with fluoride), is low, so it is difficult to selectively remove trace concentration of fluoride from actual solutions using usual anion-exchange resins. It has therefore been proposed to use cation-exchange resins loaded with high-valency metal ions, such as tri- and tetravalent metal ions [4]. **Figure 1** shows, as an example, the mechanism of adsorption of arsenate on a sulfonic acid-type cation-exchange resin loaded with trivalent ferric ion. In this case, all three positive charges of the ferric ion cannot be neutralized only by the sulfonic acid functional groups (–SO3 <sup>−</sup>) due to strong steric hindrance of the cross-linked polymer matrix; one or two positive charges are neutralized by anionic species present in aqueous solution, such as hydroxyl ions, which are substituted by the anionic species in question, such as arsenate or fluoride anions. Consequently, the adsorption and desorption of these anionic species are controlled by the pH values of the aqueous solution.

However, ion-exchange resins, which are highly porous materials, suffer from some drawbacks. One disadvantage is clogging of micropores of the resins by fine particles present in actual solutions, making the smooth operation in packed columns difficult; another issue is cracking of the resin, caused by numerous cycles of fluctuations in pH and solute concentrations over long periods of operation, like weathering of rocks. In such cases, the resins are wasted.

In our research, we attempted to develop an inexpensive removal technique for fluoride that is free from the above-mentioned troubles by using waste materials. In this work, biomass wastes such as orange juice residue [5, 6] and waste seaweeds [7] and spent cation-exchange resins [8] were employed. This study also aimed to find effective uses of waste materials to support the sustainable development of nearfuture society.

**125**

**Figure 2.**

*Chemical structures of pectin, pectic acid, and alginic acid.*

*Adsorptive Removal of Fluoride onto Different Waste Materials: Orange Juice Residue, Waste…*

Orange juice is produced from whole oranges by mechanical peeling followed by juicing processes. Approximately, half of each orange is left as orange juice residue, abbreviated as OJR hereafter, which consists of thick outer rind, thin inner peel, seeds, and calyces. Currently, OJR is used as cattle feed and fertilizer in Japan. Its main components are polysaccharides, such as cellulose and pectin, partly methylesterified pectic acid, the chemical structures of which are shown in **Figure 2**,

To prepare the adsorption gel and improve its adsorption capacity for metal ions, OJR was treated with calcium hydroxide to increase the content of carboxylic acid groups, which are the adsorption sites for cationic metal ions. Saponification of the methyl-ester parts of pectin was carried out according to the reaction shown in

For example, about 100 g OJR obtained just after juicing, kindly donated by JA Saga Beverage Co. Ltd., was added to a juicer with 8 g calcium hydroxide, and the sample was pulverized. The resulting mixture was transferred to a beaker, along with a large volume of water, and the mixture was stirred for 24 h at 200 rpm and room temperature to facilitate the saponification reaction. The initial pH of the mixture was maintained at around 12.5 by adding sodium hydroxide solution. After decantation, the mixture was repeatedly washed using water and decanted until

*DOI: http://dx.doi.org/10.5772/intechopen.80448*

**Figure 3** [5].

**2. Preparation of adsorbents for fluoride removal**

**2.1 Preparation of adsorbents from orange juice residue**

together with alginic acid, which is mentioned in Section 2.2.

#### **Figure 1.**

*Mechanism of adsorption of anionic species on cation-exchange resins loaded with high-valency metal ions (example of adsorption of arsenate ion on sulfonic acid type of strongly acidic cation-exchange resin loaded with ferric ion).*

*Adsorptive Removal of Fluoride onto Different Waste Materials: Orange Juice Residue, Waste… DOI: http://dx.doi.org/10.5772/intechopen.80448*

## **2. Preparation of adsorbents for fluoride removal**

*Environmental Chemistry and Recent Pollution Control Approaches*

centration to less than 8 mg dm<sup>−</sup><sup>3</sup>

the sulfonic acid functional groups (–SO3

weathering of rocks. In such cases, the resins are wasted.

values of the aqueous solution.

future society.

10 mg dm<sup>−</sup><sup>3</sup>

1.5 mg dm<sup>−</sup><sup>3</sup>

(Ksp = 3.9 × 10<sup>−</sup>11 (e.g., see [1])), it is theoretically difficult to lower the con-

. The maximum acceptable limit of fluoride in drinking water is

meet the regulation for fluoride before discharging industrial waste solutions into the environment. Adsorption techniques, including ion-exchange, are most suitable to remove such trace concentrations of contaminants in water. According to the well-known Hoffmeister's selectivity series of anion-exchange [3], the selectivity of usual anion-exchange resins for fluoride over other anionic species, such as sulfate and chloride (which usually coexist together with fluoride), is low, so it is difficult to selectively remove trace concentration of fluoride from actual solutions using usual anion-exchange resins. It has therefore been proposed to use cation-exchange resins loaded with high-valency metal ions, such as tri- and tetravalent metal ions [4]. **Figure 1** shows, as an example, the mechanism of adsorption of arsenate on a sulfonic acid-type cation-exchange resin loaded with trivalent ferric ion. In this case, all three positive charges of the ferric ion cannot be neutralized only by

cross-linked polymer matrix; one or two positive charges are neutralized by anionic species present in aqueous solution, such as hydroxyl ions, which are substituted by the anionic species in question, such as arsenate or fluoride anions. Consequently, the adsorption and desorption of these anionic species are controlled by the pH

However, ion-exchange resins, which are highly porous materials, suffer from some drawbacks. One disadvantage is clogging of micropores of the resins by fine particles present in actual solutions, making the smooth operation in packed columns difficult; another issue is cracking of the resin, caused by numerous cycles of fluctuations in pH and solute concentrations over long periods of operation, like

In our research, we attempted to develop an inexpensive removal technique for fluoride that is free from the above-mentioned troubles by using waste materials. In this work, biomass wastes such as orange juice residue [5, 6] and waste seaweeds [7] and spent cation-exchange resins [8] were employed. This study also aimed to find effective uses of waste materials to support the sustainable development of near-

*Mechanism of adsorption of anionic species on cation-exchange resins loaded with high-valency metal ions (example of adsorption of arsenate ion on sulfonic acid type of strongly acidic cation-exchange resin loaded* 

(e.g., see [2]). Consequently, some additional treatment is necessary to

and practically difficult to achieve less than

<sup>−</sup>) due to strong steric hindrance of the

**124**

**Figure 1.**

*with ferric ion).*

## **2.1 Preparation of adsorbents from orange juice residue**

Orange juice is produced from whole oranges by mechanical peeling followed by juicing processes. Approximately, half of each orange is left as orange juice residue, abbreviated as OJR hereafter, which consists of thick outer rind, thin inner peel, seeds, and calyces. Currently, OJR is used as cattle feed and fertilizer in Japan. Its main components are polysaccharides, such as cellulose and pectin, partly methylesterified pectic acid, the chemical structures of which are shown in **Figure 2**, together with alginic acid, which is mentioned in Section 2.2.

To prepare the adsorption gel and improve its adsorption capacity for metal ions, OJR was treated with calcium hydroxide to increase the content of carboxylic acid groups, which are the adsorption sites for cationic metal ions. Saponification of the methyl-ester parts of pectin was carried out according to the reaction shown in **Figure 3** [5].

For example, about 100 g OJR obtained just after juicing, kindly donated by JA Saga Beverage Co. Ltd., was added to a juicer with 8 g calcium hydroxide, and the sample was pulverized. The resulting mixture was transferred to a beaker, along with a large volume of water, and the mixture was stirred for 24 h at 200 rpm and room temperature to facilitate the saponification reaction. The initial pH of the mixture was maintained at around 12.5 by adding sodium hydroxide solution. After decantation, the mixture was repeatedly washed using water and decanted until

**Figure 2.** *Chemical structures of pectin, pectic acid, and alginic acid.*

**Figure 3.** *Saponification of methyl-ester parts of pectin with calcium hydroxide.*

it reached neutral pH. In this process, water washing is important because OJR contains citric acid, which functions as a water-soluble chelating agent, impeding adsorption of metal ions or eluting the loaded metal ions. Finally, the mixture was filtered to obtain a wet gel, which was dried in a convection oven for about 48 h at 70°C to obtain dry gel. The prepared dry gel is referred to as saponified OJR gel (SOJR gel). The specific surface area of this gel was measured as 7.25 m<sup>2</sup> g<sup>−</sup><sup>1</sup> . **Figure 4** shows the outline of the preparation route of SOJR gel and metal-loaded SOJR gel (zirconium(IV)-loaded SOJR gel, in this case), which will be mentioned later.

**Figure 5** shows an image of scanning electron microscope of thus prepared SOJR gel. As seen from this figure, SOJR gel is not a porous material.

## **2.2 Preparation of adsorbents from waste seaweeds**

In recent years, big cities adjacent to seas in Japan have been suffering from pollution of their sea sides by waste seaweeds, *Ulva japonica* in particular, caused by their overgrowth due to the eutrophication of the seas around these cities. Large amount of these seaweeds decay on beaches in summer and generating stench; consequently, the treatment of the seaweed wastes has become a serious environmental problem for municipalities of these coastal areas. The development of effective uses of these waste seaweeds is strongly required in Japan. The *Ulva* species of seaweed contains a high content of polysaccharides, including alginic acid (15–65%), lignin

**127**

**Figure 6.**

structure.

**Figure 5.**

*Adsorptive Removal of Fluoride onto Different Waste Materials: Orange Juice Residue, Waste…*

(1–3%), protein (6–15%), lipid (1–4%), other amino acids, minerals, and watersoluble organics [9]. Alginic acid presents as calcium alginate with an egg-box

In the present work [7], a sample of *Ulva japonica* collected at Wajiro coast in Fukuoka city, Japan, was washed several times with tap water followed by distilled water to remove impurities. It was pulverized after drying in a convection oven at 70°C for 24 h and sieved to a particle size of <100 μm. The material was then cross-linked with calcium chloride to lower its aqueous solubility. The cross-linked product was washed several times with distilled water and dried in a convection oven at 70°C. Thus, prepared waste seaweed gel is termed as cross-linked seaweed and abbreviated as CSW, hereafter. Similar to the case of SOJR gel, mentioned in Section 2.1, high-valency metal ions, such as zirconium(IV), were loaded on CSW

Ion-exchange resins are extensively used in a variety of field, such as water softening, wastewater treatment, precious metal recovery, food industries, and

*Preparation of metal-loaded cross-linked seaweed (CSW) gel for fluoride removal [M = Zr(IV), La(III)].*

to develop adsorption sites for fluoride, as shown in **Figure 6**.

**2.3 Preparation of adsorbents from spent cation-exchange resin**

*DOI: http://dx.doi.org/10.5772/intechopen.80448*

*Scanning electron microscope image of SOJR gel.*

#### **Figure 4.** *Preparation route of adsorption gels from OJR.*

*Adsorptive Removal of Fluoride onto Different Waste Materials: Orange Juice Residue, Waste… DOI: http://dx.doi.org/10.5772/intechopen.80448*

**Figure 5.** *Scanning electron microscope image of SOJR gel.*

*Environmental Chemistry and Recent Pollution Control Approaches*

*Saponification of methyl-ester parts of pectin with calcium hydroxide.*

it reached neutral pH. In this process, water washing is important because OJR contains citric acid, which functions as a water-soluble chelating agent, impeding adsorption of metal ions or eluting the loaded metal ions. Finally, the mixture was filtered to obtain a wet gel, which was dried in a convection oven for about 48 h at 70°C to obtain dry gel. The prepared dry gel is referred to as saponified OJR gel (SOJR gel). The specific surface area of this gel was measured as 7.25 m<sup>2</sup>

**Figure 4** shows the outline of the preparation route of SOJR gel and metal-loaded SOJR gel (zirconium(IV)-loaded SOJR gel, in this case), which will be mentioned

In recent years, big cities adjacent to seas in Japan have been suffering from pollution of their sea sides by waste seaweeds, *Ulva japonica* in particular, caused by their overgrowth due to the eutrophication of the seas around these cities. Large amount of these seaweeds decay on beaches in summer and generating stench; consequently, the treatment of the seaweed wastes has become a serious environmental problem for municipalities of these coastal areas. The development of effective uses of these waste seaweeds is strongly required in Japan. The *Ulva* species of seaweed contains a high content of polysaccharides, including alginic acid (15–65%), lignin

gel. As seen from this figure, SOJR gel is not a porous material.

**2.2 Preparation of adsorbents from waste seaweeds**

**Figure 5** shows an image of scanning electron microscope of thus prepared SOJR

 g<sup>−</sup><sup>1</sup> .

**126**

**Figure 4.**

*Preparation route of adsorption gels from OJR.*

later.

**Figure 3.**

(1–3%), protein (6–15%), lipid (1–4%), other amino acids, minerals, and watersoluble organics [9]. Alginic acid presents as calcium alginate with an egg-box structure.

In the present work [7], a sample of *Ulva japonica* collected at Wajiro coast in Fukuoka city, Japan, was washed several times with tap water followed by distilled water to remove impurities. It was pulverized after drying in a convection oven at 70°C for 24 h and sieved to a particle size of <100 μm. The material was then cross-linked with calcium chloride to lower its aqueous solubility. The cross-linked product was washed several times with distilled water and dried in a convection oven at 70°C. Thus, prepared waste seaweed gel is termed as cross-linked seaweed and abbreviated as CSW, hereafter. Similar to the case of SOJR gel, mentioned in Section 2.1, high-valency metal ions, such as zirconium(IV), were loaded on CSW to develop adsorption sites for fluoride, as shown in **Figure 6**.

## **2.3 Preparation of adsorbents from spent cation-exchange resin**

Ion-exchange resins are extensively used in a variety of field, such as water softening, wastewater treatment, precious metal recovery, food industries, and

catalytic processes. Although ion-exchange resins can be regenerated numerous times, they gradually deteriorate owing to the generation of many cracks, which impede smooth column operation and become unusable after many cycles of adsorption followed by elution as mentioned earlier. Tons of spent ion-exchange resins are discarded every year all over the world. Although they are unsuitable for column operation, their functional groups are still active; however, ideas for effective reutilization of such spent ion-exchange resins have not been proposed to date.

In our study [8], we attempted to effectively use such spent ion-exchange resins by pulverizing them into fine powders for use in batch operation together with a coagulating agent, that is, by means of the combined processes of adsorption and coagulation. A sample of spent cation-exchange resin containing sulfonic acid functional groups was pulverized into fine powders and converted to an anion exchanger by loading Zr(IV) ions for fluoride ion removal. The feasibility of using spent resin powder after loading Zr(IV) as ligand exchange-type material for fluoride adsorption was tested in combination with a coagulating agent in a batch system.

A sample of spent strongly acidic cation-exchange resin, MUROMAC MBX8-WH, which had been employed for the production of ion-exchange water, was kindly supplied by Muromachi Chemical Co. Ltd., Omuta, Japan. The polymer matrix of this resin is polystyrene cross-linked by divinylbenzene and it contained functional groups of sulfonic acid. The sample was pulverized into a fine powder, the average diameter of which was less than 20 μm. Thus, prepared resin powder is abbreviated as SRP hereafter. Because of the presence of an exchangeable hydrogen ion in the sulfonic acid group, waste resin powder can effectively adsorb cationic species of metal ions, such as Cu(II), Cd(II), Fe(III), La(III), and Zr(IV), whereas it has low affinity toward anionic species like fluoride ion. Similar to the cases of SOJR and CSW, the adsorption sites for fluoride anion were developed by loading Zr(IV) ion onto the SRP. Here, Zr(IV) was loaded by replacing the hydrogen ion from sulfonic acid functional groups of SRP by the cation-exchange mechanism as shown in **Figure 7**. The material obtained in this way is termed Zr(IV)-loaded spent resin powder and abbreviated as Zr-SRP hereafter.

#### **Figure 7.**

*Development of active sites for fluoride onto spent resin powder (SRP) containing sulfonic acid functional group via. Zr(IV) loading.*

**129**

**Figure 8.**

*loaded with various high-valency metal ions.*

*Adsorptive Removal of Fluoride onto Different Waste Materials: Orange Juice Residue, Waste…*

**3. Adsorption behavior of fluoride on saponified orange juice residue** 

**Figure 8** shows the effect of equilibrium pH on the adsorption of fluoride on SOJR gels loaded with various high-valency metal ions. It is apparent that pH greatly influenced the adsorption in the presence of the different metal ions, although the adsorption decreases with increasing pH, regardless of the loaded metal ion. Of the metal ions tested, Zr(IV) exhibits the most effective adsorption, at low pH in particular. The decrease in adsorption at high pH is attributed to the effect of hydroxyl ions, which compete with fluoride ion for adsorption sites on SOJR gel, as depicted in **Figure 9** for the case of Zr(IV)-loaded SOJR gel.

Also from this figure, it is apparent that the adsorption and desorption of

**Figure 11** shows the effect of coexisting species on the adsorption of fluoride. Although sulfate most effectively interferes with the adsorption of fluoride, it is only less than 2%; consequently, the effect of coexisting species was practically negligible, that is, Zr(IV)-loaded SOJR gel exhibited high selectivity to fluoride over coexisting species. Similar was observed also in the adsorption on Zr(IV)-loaded other adsorbents. **Figure 12** shows time variation in the adsorption of fluoride on Zr(IV)-loaded SOJR gel at various temperatures. Equilibrium was attained within a short contact time (shorter than 100 min), indicating rapid adsorption, regardless of temperature. **Figure 13** shows the effect of initial pH on the elution of fluoride adsorbed on Zr(IV)-loaded SOJR gel. The adsorbed fluoride was quantitatively eluted at pH

*Effect of equilibrium pH (pHe) on the adsorption of fluoride on saponified orange juice residue (SOJR) gels* 

**Figure 10** shows the adsorption isotherms of fluoride, which is the relationship between the amount of adsorbed fluoride (q) and the fluoride concentration (Ce) in the aqueous solution at equilibrium, on SOJR gels loaded with various highvalency metal ions at 30°C. It is evident that SOJR gel loaded with Zr(IV) exhibited the highest adsorption capacity for fluoride. Consequently, we used Zr(IV)-loaded

**gels loaded with various high-valency metal ions**

*DOI: http://dx.doi.org/10.5772/intechopen.80448*

fluoride can be easily controlled by changing pH.

adsorbent in subsequent work.

higher than 12.

*Adsorptive Removal of Fluoride onto Different Waste Materials: Orange Juice Residue, Waste… DOI: http://dx.doi.org/10.5772/intechopen.80448*

## **3. Adsorption behavior of fluoride on saponified orange juice residue gels loaded with various high-valency metal ions**

**Figure 8** shows the effect of equilibrium pH on the adsorption of fluoride on SOJR gels loaded with various high-valency metal ions. It is apparent that pH greatly influenced the adsorption in the presence of the different metal ions, although the adsorption decreases with increasing pH, regardless of the loaded metal ion. Of the metal ions tested, Zr(IV) exhibits the most effective adsorption, at low pH in particular. The decrease in adsorption at high pH is attributed to the effect of hydroxyl ions, which compete with fluoride ion for adsorption sites on SOJR gel, as depicted in **Figure 9** for the case of Zr(IV)-loaded SOJR gel.

Also from this figure, it is apparent that the adsorption and desorption of fluoride can be easily controlled by changing pH.

**Figure 10** shows the adsorption isotherms of fluoride, which is the relationship between the amount of adsorbed fluoride (q) and the fluoride concentration (Ce) in the aqueous solution at equilibrium, on SOJR gels loaded with various highvalency metal ions at 30°C. It is evident that SOJR gel loaded with Zr(IV) exhibited the highest adsorption capacity for fluoride. Consequently, we used Zr(IV)-loaded adsorbent in subsequent work.

**Figure 11** shows the effect of coexisting species on the adsorption of fluoride. Although sulfate most effectively interferes with the adsorption of fluoride, it is only less than 2%; consequently, the effect of coexisting species was practically negligible, that is, Zr(IV)-loaded SOJR gel exhibited high selectivity to fluoride over coexisting species. Similar was observed also in the adsorption on Zr(IV)-loaded other adsorbents.

**Figure 12** shows time variation in the adsorption of fluoride on Zr(IV)-loaded SOJR gel at various temperatures. Equilibrium was attained within a short contact time (shorter than 100 min), indicating rapid adsorption, regardless of temperature.

**Figure 13** shows the effect of initial pH on the elution of fluoride adsorbed on Zr(IV)-loaded SOJR gel. The adsorbed fluoride was quantitatively eluted at pH higher than 12.

#### **Figure 8.**

*Environmental Chemistry and Recent Pollution Control Approaches*

catalytic processes. Although ion-exchange resins can be regenerated numerous times, they gradually deteriorate owing to the generation of many cracks, which impede smooth column operation and become unusable after many cycles of adsorption followed by elution as mentioned earlier. Tons of spent ion-exchange resins are discarded every year all over the world. Although they are unsuitable for column operation, their functional groups are still active; however, ideas for effective reutilization of such spent ion-exchange resins have not been proposed

In our study [8], we attempted to effectively use such spent ion-exchange resins by pulverizing them into fine powders for use in batch operation together with a coagulating agent, that is, by means of the combined processes of adsorption and coagulation. A sample of spent cation-exchange resin containing sulfonic acid functional groups was pulverized into fine powders and converted to an anion exchanger by loading Zr(IV) ions for fluoride ion removal. The feasibility of using spent resin powder after loading Zr(IV) as ligand exchange-type material for fluoride adsorption was tested in combination with a coagulating agent in a

A sample of spent strongly acidic cation-exchange resin, MUROMAC MBX8-WH, which had been employed for the production of ion-exchange water, was kindly supplied by Muromachi Chemical Co. Ltd., Omuta, Japan. The polymer matrix of this resin is polystyrene cross-linked by divinylbenzene and it contained functional groups of sulfonic acid. The sample was pulverized into a fine powder, the average diameter of which was less than 20 μm. Thus, prepared resin powder is abbreviated as SRP hereafter. Because of the presence of an exchangeable hydrogen ion in the sulfonic acid group, waste resin powder can effectively adsorb cationic species of metal ions, such as Cu(II), Cd(II), Fe(III), La(III), and Zr(IV), whereas it has low affinity toward anionic species like fluoride ion. Similar to the cases of SOJR and CSW, the adsorption sites for fluoride anion were developed by loading Zr(IV) ion onto the SRP. Here, Zr(IV) was loaded by replacing the hydrogen ion from sulfonic acid functional groups of SRP by the cation-exchange mechanism as shown in **Figure 7**. The material obtained in this way is termed Zr(IV)-loaded spent resin powder and abbreviated

*Development of active sites for fluoride onto spent resin powder (SRP) containing sulfonic acid functional* 

**128**

**Figure 7.**

*group via. Zr(IV) loading.*

to date.

batch system.

as Zr-SRP hereafter.

*Effect of equilibrium pH (pHe) on the adsorption of fluoride on saponified orange juice residue (SOJR) gels loaded with various high-valency metal ions.*

**Figure 9.**

*Adsorption and desorption mechanism of fluoride on Zr(IV)-loaded saponified orange juice residue (SOJR) gels.*

#### **Figure 10.**

*Adsorption isotherms of fluoride on saponified orange juice residue (SOJR) gels loaded with various highvalency metal ions at 30°C.*

**Figure 11.**

*Effect of coexisting species in the aqueous solution on adsorption of fluoride on Zr(IV)-loaded saponified orange juice residue (SOJR) gel.*

**131**

**Figure 13.**

**Figure 12.**

*(SOJR) gel at various temperatures.*

cation-exchange mechanism.

SOJR gel exhibited high durability.

*Adsorptive Removal of Fluoride onto Different Waste Materials: Orange Juice Residue, Waste…*

*Time variation in the amount of adsorption of fluoride (q) on Zr(IV)-loaded saponified orange juice residue* 

**Figure 14** shows effect of initial fluoride concentration at various pH values on leakage of the loaded zirconium(IV) from the SOJR gel. Such leakage, which would cause degradation of the adsorbent, was practically negligible at all pH values, except below pH 3, where the loaded metal ions are replaced by hydrogen ions by

*Effect of pH on elution of fluoride adsorbed on Zr(IV)-loaded saponified orange juice residue (SOJR) gel.*

**Figure 15** shows the result of cycle test of adsorption of fluoride on Zr(IV)-

that the adsorption and desorption behaviors of fluoride on this gel were not significantly degraded, even after 10 cycles of adsorption and elution. The Zr(IV)-loaded

NaOH. It can be concluded

loaded SOJR gel followed by elution using 0.1 mol dm<sup>−</sup><sup>3</sup>

*DOI: http://dx.doi.org/10.5772/intechopen.80448*

*Adsorptive Removal of Fluoride onto Different Waste Materials: Orange Juice Residue, Waste… DOI: http://dx.doi.org/10.5772/intechopen.80448*

**Figure 12.**

*Environmental Chemistry and Recent Pollution Control Approaches*

*Adsorption and desorption mechanism of fluoride on Zr(IV)-loaded saponified orange juice residue (SOJR)* 

**130**

**Figure 11.**

**Figure 10.**

*valency metal ions at 30°C.*

**Figure 9.**

*gels.*

*orange juice residue (SOJR) gel.*

*Effect of coexisting species in the aqueous solution on adsorption of fluoride on Zr(IV)-loaded saponified* 

*Adsorption isotherms of fluoride on saponified orange juice residue (SOJR) gels loaded with various high-*

*Time variation in the amount of adsorption of fluoride (q) on Zr(IV)-loaded saponified orange juice residue (SOJR) gel at various temperatures.*

*Effect of pH on elution of fluoride adsorbed on Zr(IV)-loaded saponified orange juice residue (SOJR) gel.*

**Figure 14** shows effect of initial fluoride concentration at various pH values on leakage of the loaded zirconium(IV) from the SOJR gel. Such leakage, which would cause degradation of the adsorbent, was practically negligible at all pH values, except below pH 3, where the loaded metal ions are replaced by hydrogen ions by cation-exchange mechanism.

**Figure 15** shows the result of cycle test of adsorption of fluoride on Zr(IV) loaded SOJR gel followed by elution using 0.1 mol dm<sup>−</sup><sup>3</sup> NaOH. It can be concluded that the adsorption and desorption behaviors of fluoride on this gel were not significantly degraded, even after 10 cycles of adsorption and elution. The Zr(IV)-loaded SOJR gel exhibited high durability.

**Figure 14.**

*Effect of initial fluoride concentration of fluoride at various pH values on leakage of loaded zirconium(IV) from saponified orange juice residue (SOJR) gel.*

**Figure 15.**

*Effect of number of cycles of adsorption of fluoride on Zr(IV)-loaded saponified orange juice residue (SOJR) gel followed by elution using 0.1 mol dm<sup>−</sup><sup>3</sup> NaOH.*

## **4. Adsorption behavior of fluoride on waste seaweed gel loaded with various high-valent metal ions**

**Figure 16** shows the effect of equilibrium pH on the adsorption of fluoride on the cross-linked seaweed gel (CSW) and CSW gels loaded with Zr(IV) and La(III). Unloaded CSW gel also exhibits some adsorption of fluoride, which is attributable to calcium(II) ion contained in seaweed as calcium alginate. Similar to SOJR gel, the adsorption of fluoride was greatly improved by loading high-valency metal ions, of which Zr(IV) exhibited better adsorption than La(III). The decrease in adsorption

**133**

**Figure 17.**

*Adsorptive Removal of Fluoride onto Different Waste Materials: Orange Juice Residue, Waste…*

with increasing pH at high pH is attributable to the competition of fluoride ion with hydroxyl ion for adsorption sites on the loaded metal ions; that is, the adsorption and desorption mechanism in this system can also be reasonably interpreted by that

*Effect of equilibrium pH on the adsorption of fluoride on the cross-linked seaweed gel (CSW) and metal-*

**Figure 17** shows the effect of initial pH on leakage of the loaded metal ions. It is apparent that, compared with La(III), the loaded Zr(IV) is much more difficult to leak from CSW than La(III); that is, Zr(IV) is also more suitable as the loaded metal

*Effect of initial pH on leakage of the loaded metal ions from cross-linked seaweed (CSW) gels.*

*DOI: http://dx.doi.org/10.5772/intechopen.80448*

depicted in **Figure 9** for SOJR gel.

ion on CSW.

**Figure 16.**

*loaded CSW gels [7].*

*Adsorptive Removal of Fluoride onto Different Waste Materials: Orange Juice Residue, Waste… DOI: http://dx.doi.org/10.5772/intechopen.80448*

#### **Figure 16.**

*Environmental Chemistry and Recent Pollution Control Approaches*

**4. Adsorption behavior of fluoride on waste seaweed gel loaded with** 

 *NaOH.*

*Effect of number of cycles of adsorption of fluoride on Zr(IV)-loaded saponified orange juice residue (SOJR)* 

*Effect of initial fluoride concentration of fluoride at various pH values on leakage of loaded zirconium(IV)* 

**Figure 16** shows the effect of equilibrium pH on the adsorption of fluoride on the cross-linked seaweed gel (CSW) and CSW gels loaded with Zr(IV) and La(III). Unloaded CSW gel also exhibits some adsorption of fluoride, which is attributable to calcium(II) ion contained in seaweed as calcium alginate. Similar to SOJR gel, the adsorption of fluoride was greatly improved by loading high-valency metal ions, of which Zr(IV) exhibited better adsorption than La(III). The decrease in adsorption

**various high-valent metal ions**

*gel followed by elution using 0.1 mol dm<sup>−</sup><sup>3</sup>*

*from saponified orange juice residue (SOJR) gel.*

**132**

**Figure 15.**

**Figure 14.**

*Effect of equilibrium pH on the adsorption of fluoride on the cross-linked seaweed gel (CSW) and metalloaded CSW gels [7].*

with increasing pH at high pH is attributable to the competition of fluoride ion with hydroxyl ion for adsorption sites on the loaded metal ions; that is, the adsorption and desorption mechanism in this system can also be reasonably interpreted by that depicted in **Figure 9** for SOJR gel.

**Figure 17** shows the effect of initial pH on leakage of the loaded metal ions. It is apparent that, compared with La(III), the loaded Zr(IV) is much more difficult to leak from CSW than La(III); that is, Zr(IV) is also more suitable as the loaded metal ion on CSW.

**Figure 17.** *Effect of initial pH on leakage of the loaded metal ions from cross-linked seaweed (CSW) gels.*

## **5. Adsorption behavior of fluoride on pulverized spent cation-exchange resin loaded with zirconium(IV) ions**

A small amount of commercially available inorganic coagulating agent, MAGNETITE III, the main components of which are calcium, aluminum, and iron, was added with Zr-SRP to test solutions containing trace concentration of fluoride to achieve smooth solid/liquid separation or smooth filtration. The coagulating agent is abbreviated as CA, hereafter. It was found that stable floc was formed at a CA/Zr-SRP ratio higher than 0.2.

**Figure 18** shows the effect of equilibrium pH on the adsorption of fluoride onto SRP before and after Zr(IV) loading in the presence and absence of CA. Although SRP exhibited only negligible adsorption for fluoride, the adsorption was greatly

#### **Figure 18.**

*Effect of equilibrium pH on adsorption of fluoride on pulverized spent cation-exchange resin (SRP) before and after Zr(IV) loading [8].*

#### **Figure 19.**

*Effect of interfering anionic species on adsorption of fluoride on Zr(IV)-loaded pulverized spent cationexchange resin (Zr-SRP) [8].*

**135**

**Figure 21.**

**Figure 20.**

*Adsorptive Removal of Fluoride onto Different Waste Materials: Orange Juice Residue, Waste…*

*Effect of fluoride concentration on leakage of loaded Zr(IV) from Zr(IV)-loaded pulverized spent cation-*

improved by loading Zr(IV), similar to the cases of SOJR and CSW. The small

affected by the addition of small amount of CA.

*spent cation-exchange resin (Zr-SRP) [8].*

amount of adsorption on unloaded SRP at pH = 4–6 is considered to be due to calcium accumulated in the resin during its previous function in water treatment. Adsorption of fluoride also rapidly decreased with increasing pH at pH values above 6, similar to the cases of SOJR and CSW, which is attributable to the competition of fluoride ions with hydroxyl ions for the adsorption sites on Zr-SRP. Adsorption of fluoride was not

*Effect of concentration of sodium hydroxide on the elution of fluoride adsorbed on Zr(IV)-loaded pulverized* 

*DOI: http://dx.doi.org/10.5772/intechopen.80448*

*exchange resin (Zr-SRP) at various pH values [8].*

*Adsorptive Removal of Fluoride onto Different Waste Materials: Orange Juice Residue, Waste… DOI: http://dx.doi.org/10.5772/intechopen.80448*

**Figure 20.**

*Environmental Chemistry and Recent Pollution Control Approaches*

**resin loaded with zirconium(IV) ions**

CA/Zr-SRP ratio higher than 0.2.

**5. Adsorption behavior of fluoride on pulverized spent cation-exchange** 

**Figure 18** shows the effect of equilibrium pH on the adsorption of fluoride onto SRP before and after Zr(IV) loading in the presence and absence of CA. Although SRP exhibited only negligible adsorption for fluoride, the adsorption was greatly

*Effect of equilibrium pH on adsorption of fluoride on pulverized spent cation-exchange resin (SRP) before and* 

*Effect of interfering anionic species on adsorption of fluoride on Zr(IV)-loaded pulverized spent cation-*

A small amount of commercially available inorganic coagulating agent, MAGNETITE III, the main components of which are calcium, aluminum, and iron, was added with Zr-SRP to test solutions containing trace concentration of fluoride to achieve smooth solid/liquid separation or smooth filtration. The coagulating agent is abbreviated as CA, hereafter. It was found that stable floc was formed at a

**134**

**Figure 19.**

**Figure 18.**

*after Zr(IV) loading [8].*

*exchange resin (Zr-SRP) [8].*

*Effect of fluoride concentration on leakage of loaded Zr(IV) from Zr(IV)-loaded pulverized spent cationexchange resin (Zr-SRP) at various pH values [8].*

**Figure 21.**

*Effect of concentration of sodium hydroxide on the elution of fluoride adsorbed on Zr(IV)-loaded pulverized spent cation-exchange resin (Zr-SRP) [8].*

improved by loading Zr(IV), similar to the cases of SOJR and CSW. The small amount of adsorption on unloaded SRP at pH = 4–6 is considered to be due to calcium accumulated in the resin during its previous function in water treatment. Adsorption of fluoride also rapidly decreased with increasing pH at pH values above 6, similar to the cases of SOJR and CSW, which is attributable to the competition of fluoride ions with hydroxyl ions for the adsorption sites on Zr-SRP. Adsorption of fluoride was not affected by the addition of small amount of CA.

#### **Figure 22.**

*Effect of number of cycles of adsorption of fluoride on Zr(IV)-loaded pulverized spent cation-exchange resin (Zr-SRP) followed by elution using 0.1 Mol dm<sup>−</sup><sup>3</sup> NaOH solution [8].*

**Figure 19** shows the effect of interfering anionic species (chloride, nitrate, and sulfate) present in aqueous fluoride solutions on the adsorption of fluoride on Zr-SRP. Also in this case, the effect of coexisting anionic species was relatively low.

**Figure 20** shows leakage of Zr(IV) from Zr-SRP by varying concentration of fluoride at various pH values. It is evident that the leakage was negligible at pH values higher than 6, regardless of fluoride concentration.

**Figure 21** shows effect of sodium hydroxide concentration on the elution of fluoride adsorbed on Zr-SRP. The results suggest that nearly quantitative elution of fluoride can be achieved by 0.1 mol dm<sup>−</sup><sup>3</sup> sodium hydroxide solution also in this case.

**Figure 22** shows the result of durability test of Zr-SRP for repeating adsorption of fluoride followed by elution for up to 6 cycles. This figure suggests that Zr-SRP is not significantly degraded up to at least 6 cycles.

## **6. Comparison of adsorption capacities for fluoride on Zr(IV)-loaded adsorbents prepared from wastes**

Adsorbents are evaluated in terms of their maximum adsorption capacities and selectivity for targeted species over other coexisting species. Selectivity for fluoride of three adsorbents prepared from wastes over other anionic species is discussed in the preceding sections. In this section, the maximum adsorption capacities on Zr(IV)-loaded SOJR, CSW, and SRP for fluoride were compared.

**Figure 23** shows adsorption isotherms for fluoride on Zr(IV)-loaded SOJR, CSW, and SRP at 30°C. For all of these adsorbents, the adsorption amount increased with increasing fluoride concentration in the low concentration range and tends to approach a constant value for each adsorbent in the high concentration range, suggesting typical Langmuir-type adsorption.

These adsorption isotherms were therefore replotted according to the Langmuir equation, expressed by Eq. (1) as shown in **Figure 24**.

**137**

**Figure 24.**

**Figure 23.**

*Adsorptive Removal of Fluoride onto Different Waste Materials: Orange Juice Residue, Waste…*

Ce/q = 1/qmaxb + Ce/qmax (1)

where qmax and b denote the maximum adsorption capacity and adsorption equilibrium constant, respectively, based on the Langmuir's monolayer adsorption theory. As expected from Eq. (1), the plots in **Figure 24** lay on straight lines. From the values of intercepts of these straight lines with the ordinate and their slopes, the

*Adsorption isotherms of fluoride on Zr(IV)-loaded saponified orange juice residue (SOJR), cross-linked* 

02468

**Ce [mmol/dm3]**

*seaweed (CSW) gels, and pulverized spent cation-exchange resin (SRP) at 30°C.*

Zr(IV)-SRP Zr(IV)-SOJR Zr(IV)-CSW

0

*Replots of* **Figure 23** *according to Eq. (1), the Langmuir's equation.*

2

**Ce/qe [g/d**

**m3]**

4

6

*DOI: http://dx.doi.org/10.5772/intechopen.80448*

*Adsorptive Removal of Fluoride onto Different Waste Materials: Orange Juice Residue, Waste… DOI: http://dx.doi.org/10.5772/intechopen.80448*

$$\mathbf{Ce/q} = \mathbf{1/q}\_{\text{max}} \mathbf{b} + \mathbf{Ce/q}\_{\text{max}} \tag{1}$$

where qmax and b denote the maximum adsorption capacity and adsorption equilibrium constant, respectively, based on the Langmuir's monolayer adsorption theory.

As expected from Eq. (1), the plots in **Figure 24** lay on straight lines. From the values of intercepts of these straight lines with the ordinate and their slopes, the

#### **Figure 23.**

*Environmental Chemistry and Recent Pollution Control Approaches*

**Figure 19** shows the effect of interfering anionic species (chloride, nitrate, and sulfate) present in aqueous fluoride solutions on the adsorption of fluoride on Zr-SRP. Also in this case, the effect of coexisting anionic species was relatively low. **Figure 20** shows leakage of Zr(IV) from Zr-SRP by varying concentration of fluoride at various pH values. It is evident that the leakage was negligible at pH

*Effect of number of cycles of adsorption of fluoride on Zr(IV)-loaded pulverized spent cation-exchange resin* 

 *NaOH solution [8].*

**Figure 21** shows effect of sodium hydroxide concentration on the elution of fluoride adsorbed on Zr-SRP. The results suggest that nearly quantitative elution of

**6. Comparison of adsorption capacities for fluoride on Zr(IV)-loaded** 

Zr(IV)-loaded SOJR, CSW, and SRP for fluoride were compared.

range, suggesting typical Langmuir-type adsorption.

equation, expressed by Eq. (1) as shown in **Figure 24**.

Adsorbents are evaluated in terms of their maximum adsorption capacities and selectivity for targeted species over other coexisting species. Selectivity for fluoride of three adsorbents prepared from wastes over other anionic species is discussed in the preceding sections. In this section, the maximum adsorption capacities on

**Figure 23** shows adsorption isotherms for fluoride on Zr(IV)-loaded SOJR,

These adsorption isotherms were therefore replotted according to the Langmuir

CSW, and SRP at 30°C. For all of these adsorbents, the adsorption amount increased with increasing fluoride concentration in the low concentration range and tends to approach a constant value for each adsorbent in the high concentration

**Figure 22** shows the result of durability test of Zr-SRP for repeating adsorption of fluoride followed by elution for up to 6 cycles. This figure suggests that Zr-SRP is

sodium hydroxide solution also in this case.

values higher than 6, regardless of fluoride concentration.

fluoride can be achieved by 0.1 mol dm<sup>−</sup><sup>3</sup>

*(Zr-SRP) followed by elution using 0.1 Mol dm<sup>−</sup><sup>3</sup>*

not significantly degraded up to at least 6 cycles.

**adsorbents prepared from wastes**

**136**

**Figure 22.**

*Adsorption isotherms of fluoride on Zr(IV)-loaded saponified orange juice residue (SOJR), cross-linked seaweed (CSW) gels, and pulverized spent cation-exchange resin (SRP) at 30°C.*

**Figure 24.** *Replots of* **Figure 23** *according to Eq. (1), the Langmuir's equation.*

## *Environmental Chemistry and Recent Pollution Control Approaches*


#### **Table 1.**

*Maximum adsorption capacities and adsorption equilibrium constants of fluoride on Zr(IV)-loaded saponified orange juice residue (SOJR) and cross-linked seaweeds (CSW) gels and pulverized spent cationexchange resin (SRP) at 30°C.*


**139**

**Figure 25.**

*Adsorptive Removal of Fluoride onto Different Waste Materials: Orange Juice Residue, Waste…*

maximum adsorption capacities and adsorption equilibrium constants were evaluated, as listed in **Table 1**. The data indicate that Zr(IV)-loaded SRP exhibits the

These maximum adsorption capacities were compared with those on SOJR gel loaded with other high-valency metal ions and with those reported in literature, as listed in **Table 2**. Zr(IV)-loaded SRP and Zr(IV)-loaded SOJR exhibited higher adsorption capacities than other adsorbents, including Zr-containing adsorbents, except for READF, a commercially available porous resin that contains fine zirco-

**7. Removal tests of trace concentrations of fluoride from actual waste plating solutions using Zr(IV)-loaded adsorbents prepared from** 

On the basis of the results of fundamental adsorption tests using Zr(IV)-loaded SOJR, CSW, and SRP discussed above, adsorptive removal of trace concentrations of fluoride was tested from actual waste plating solutions using these adsorbents [6–8]. A sample of the actual waste plating solution was kindly donated by Federation of Electro Plating Industry Association, Japan, Tokyo, Japan. The

of sulfate, as well as following cationic species (mg dm<sup>−</sup><sup>3</sup>

). This figure indicates that fluoride concentration can be successfully

, the Japanese standard for fluoride, by adding only 2 g of

10.5, Fe 36.4, Cu 9.8, and Zn 1.9. Its pH value was 6.7. **Figure 25** shows the plots of fluoride concentration after the treatment using these three adsorbents as a function of S/L ratio, defined as the ratio of dry mass of added adsorbent to volume of treated solution together with the permissible level for fluoride in effluents in Japan

lowered by adding small amount of adsorbents. The concentration was reduced

*Adsorptive removal of trace concentrations of fluoride from actual waste plating solution using three adsorbents prepared in the present work, showing relationship between concentration of fluoride remained in* 

*aqueous solution after adsorption and mass of adsorbent added to unit volume of solution.*

), WHO standard for drinking water (1.5 mg/dm3

of tested sample solution.

of fluoride together with about

), and that in Japan

): Al 13.8, Ca

*DOI: http://dx.doi.org/10.5772/intechopen.80448*

nium hydroxide powder in its pores.

donated sample solutions contained 12.2 mg/dm3

highest loading capacity.

**wastes**

750 mg dm*<sup>−</sup>*<sup>3</sup>

(8 mg/dm3

(0.8 mg/dm3

to less than 0.8 mg/dm3

adsorbents to 1 dm3

#### **Table 2.**

*Maximum adsorption capacities of fluoride on various adsorbents.*

*Adsorptive Removal of Fluoride onto Different Waste Materials: Orange Juice Residue, Waste… DOI: http://dx.doi.org/10.5772/intechopen.80448*

maximum adsorption capacities and adsorption equilibrium constants were evaluated, as listed in **Table 1**. The data indicate that Zr(IV)-loaded SRP exhibits the highest loading capacity.

These maximum adsorption capacities were compared with those on SOJR gel loaded with other high-valency metal ions and with those reported in literature, as listed in **Table 2**. Zr(IV)-loaded SRP and Zr(IV)-loaded SOJR exhibited higher adsorption capacities than other adsorbents, including Zr-containing adsorbents, except for READF, a commercially available porous resin that contains fine zirconium hydroxide powder in its pores.

## **7. Removal tests of trace concentrations of fluoride from actual waste plating solutions using Zr(IV)-loaded adsorbents prepared from wastes**

On the basis of the results of fundamental adsorption tests using Zr(IV)-loaded SOJR, CSW, and SRP discussed above, adsorptive removal of trace concentrations of fluoride was tested from actual waste plating solutions using these adsorbents [6–8]. A sample of the actual waste plating solution was kindly donated by Federation of Electro Plating Industry Association, Japan, Tokyo, Japan. The donated sample solutions contained 12.2 mg/dm3 of fluoride together with about 750 mg dm*<sup>−</sup>*<sup>3</sup> of sulfate, as well as following cationic species (mg dm<sup>−</sup><sup>3</sup> ): Al 13.8, Ca 10.5, Fe 36.4, Cu 9.8, and Zn 1.9. Its pH value was 6.7. **Figure 25** shows the plots of fluoride concentration after the treatment using these three adsorbents as a function of S/L ratio, defined as the ratio of dry mass of added adsorbent to volume of treated solution together with the permissible level for fluoride in effluents in Japan (8 mg/dm3 ), WHO standard for drinking water (1.5 mg/dm3 ), and that in Japan (0.8 mg/dm3 ). This figure indicates that fluoride concentration can be successfully lowered by adding small amount of adsorbents. The concentration was reduced to less than 0.8 mg/dm3 , the Japanese standard for fluoride, by adding only 2 g of adsorbents to 1 dm3 of tested sample solution.

#### **Figure 25.**

*Adsorptive removal of trace concentrations of fluoride from actual waste plating solution using three adsorbents prepared in the present work, showing relationship between concentration of fluoride remained in aqueous solution after adsorption and mass of adsorbent added to unit volume of solution.*

*Environmental Chemistry and Recent Pollution Control Approaches*

**Adsorbents pH qmax**

Zr-impregnated cashew nut

shell carbon

**Table 1.**

*exchange resin (SRP) at 30°C.*

**(mmol/g)**

Zr(IV)-loaded SOJR 4 1.74 30 [6] Zr(IV)-loaded CSW 4 0.95 30 [7] Zr(IV)-loaded SRP 4 1.98 30 [8] Sn(IV)-loaded SOJR 3 1.18 30 [5] Ti(IV)-loaded SOJR 3 0.93 30 [5] Al(III)-loaded SOJR 6 1.03 30 [5] Fe(III)-loaded SOJR 4 0.88 30 [5] La(III)-loaded SOJR 4 1.06 30 [10] Sc(III)-loaded SOJR 4 0.60 30 [10] Sm(III)-loaded SOJR 5 1.22 30 [10] Ho(III)-loaded SOJR 5 0.93 30 [10] Ce(III)-loaded SOJR 4 0.91 30 [10] Ce(IV)-loaded SOJR 4 1.53 30 [10] READF(PG) 3 2.10 30 [11] READF(HG) 3 2.35 30 [11]

**Adsorbents qmax (mmol/g-dry weight) b (dm3**

*Maximum adsorption capacities and adsorption equilibrium constants of fluoride on Zr(IV)-loaded saponified orange juice residue (SOJR) and cross-linked seaweeds (CSW) gels and pulverized spent cation-*

Zr(IV)-loaded SOJR 1.74 3.11 Zr(IV)-loaded CSW 0.95 5.04 Zr(IV)-loaded SRP 1.98 1.18

La-loaded 200CT resin 6 1.34 30 [13] Indian FR 10 7 0.068 30 [14] Ceralite IRA 400 7 0.078 30 [14] La-loaded CL gelatin 5–7 1.12 25 [15] Nd-modified chitosan 7 1.17 30 [16] Fe-loaded cotton 4 0.97 25 [17] Protonated chitosan 7 0.38 30 [18] Activated alumina 5–6 0.86 30 [19] AFB-Pr resin 5 0.026 30 [20]

Spirogyra species IO1 7 0.05 30 [22] Waste mud 5 0.22 20 [23] Nanoaluminum hydroxide 5.2 0.17 25 [24]

Waste carbon slurry 7.5 0.23 25 [26] Montmorillonite 6 0.01 25 [27]

La-impregnated alumina 5.7–8 0.35 Room

Magnesia/chitosan composite 10 0.11 Room

*Maximum adsorption capacities of fluoride on various adsorbents.*

**Temperature (°C)**

3 0.09 30 [12]

temperature

temperature

[21]

[25]

**Reference**

**/mmol)**

**138**

**Table 2.**

## **8. Conclusion**

For the purpose of removing trace or low concentrations of fluoride from aquatic environments, novel adsorbents were prepared from three waste materials, orange juice residue, waste seaweed, and pulverized spent cation-exchange resin containing sulfonic acid functional groups, by loading with tri- or tetravalent metal ions, such as iron(III), aluminum(III), rare earths(III), and zirconium(IV). Here, the loaded metal ions function as adsorption sites and waste materials function as polymer matrices immobilizing the metal ions. The adsorption mechanisms on these adsorbents were inferred from the results of adsorption tests from aqueous solutions at various pH values. Adsorption and desorption were found to be easily controlled by changing pH. Of the high-valency metal ions tested, zirconium(IV) was found to be the most suitable as the loaded metal ion because zirconium(IV) loaded adsorbents exhibited highest adsorption of the tested metal-loaded adsorbents in the adsorption isotherm tests. Zirconium(IV)-loaded adsorbents exhibited high selectivity for fluoride over other anionic species present in aqueous solutions. Leakage of the loaded zirconium(IV) ions was found to be negligible, except at low pH, and high durability of these adsorbents was confirmed from repeated cycle tests of adsorption followed by desorption. The maximum adsorption capacities for fluoride on these adsorbents were higher than those of most adsorbents reported in literature. The removal test of trace concentration of fluoride from actual waste plating solutions revealed that the fluoride concentration could be lowered below the acceptable level by using only small amounts of these adsorbents; for example, it was reduced to less than 0.8 mg/dm3 , the Japanese standard for fluoride, by adding only 2 g of adsorbents to 1 dm3 of tested sample solution. From these results, it can be expected that trace concentration of fluoride is effectively removed by using adsorbents produced from various waste materials at cheap cost.

**141**

**Author details**

Katsutoshi Inoue1

University, Saga, Japan

provided the original work is properly cited.

\*Address all correspondence to: kanoko1921@gmail.com

© 2018 The Author(s). Licensee IntechOpen. This chapter is distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/ by/3.0), which permits unrestricted use, distribution, and reproduction in any medium,

1 Department of Applied Chemistry, Faculty of Science and Engineering, Saga

2 Central Department of Chemistry, Tribhuvan University, Kathmandu, Nepal

\*, Hari Paudyal1,2, Hidetaka Kawakita1,2 and Keisuke Ohto1

*Adsorptive Removal of Fluoride onto Different Waste Materials: Orange Juice Residue, Waste…*

of fluoride using this adsorbent is proposed as shown in **Figure 26**.

The present work was conducted in part in the project of Water-Saving Recycling Systems in 2012–2013 supported by New Energy and Industrial Development Technology Organization (NEDO). The authors acknowledge the kind donation of sample of waste plating solution by Federation of Electro Plating Industry Association, Japan, and those of pulverized spent cation-exchange resin powder and orange juice residue by Muromachi Chemical Co. Ltd., Omuta, Japan,

Although it is not noticed in laboratory-scale tests and the small-scale adsorption tests mentioned in this study, the adsorbent prepared from orange juice residue was found to generate considerable stench at larger scale, such as pilot-scale operation. Taking account of this, the adsorbent prepared from spent cation-exchange resins is recommended to be employed in commercial operations. A process for the recovery

*DOI: http://dx.doi.org/10.5772/intechopen.80448*

and JA Saga Beverage, Saga, Japan, respectively.

**Acknowledgements**

*Adsorptive Removal of Fluoride onto Different Waste Materials: Orange Juice Residue, Waste… DOI: http://dx.doi.org/10.5772/intechopen.80448*

Although it is not noticed in laboratory-scale tests and the small-scale adsorption tests mentioned in this study, the adsorbent prepared from orange juice residue was found to generate considerable stench at larger scale, such as pilot-scale operation. Taking account of this, the adsorbent prepared from spent cation-exchange resins is recommended to be employed in commercial operations. A process for the recovery of fluoride using this adsorbent is proposed as shown in **Figure 26**.

## **Acknowledgements**

*Environmental Chemistry and Recent Pollution Control Approaches*

it was reduced to less than 0.8 mg/dm3

ing only 2 g of adsorbents to 1 dm3

For the purpose of removing trace or low concentrations of fluoride from aquatic environments, novel adsorbents were prepared from three waste materials, orange juice residue, waste seaweed, and pulverized spent cation-exchange resin containing sulfonic acid functional groups, by loading with tri- or tetravalent metal ions, such as iron(III), aluminum(III), rare earths(III), and zirconium(IV). Here, the loaded metal ions function as adsorption sites and waste materials function as polymer matrices immobilizing the metal ions. The adsorption mechanisms on these adsorbents were inferred from the results of adsorption tests from aqueous solutions at various pH values. Adsorption and desorption were found to be easily controlled by changing pH. Of the high-valency metal ions tested, zirconium(IV) was found to be the most suitable as the loaded metal ion because zirconium(IV) loaded adsorbents exhibited highest adsorption of the tested metal-loaded adsorbents in the adsorption isotherm tests. Zirconium(IV)-loaded adsorbents exhibited high selectivity for fluoride over other anionic species present in aqueous solutions. Leakage of the loaded zirconium(IV) ions was found to be negligible, except at low pH, and high durability of these adsorbents was confirmed from repeated cycle tests of adsorption followed by desorption. The maximum adsorption capacities for fluoride on these adsorbents were higher than those of most adsorbents reported in literature. The removal test of trace concentration of fluoride from actual waste plating solutions revealed that the fluoride concentration could be lowered below the acceptable level by using only small amounts of these adsorbents; for example,

can be expected that trace concentration of fluoride is effectively removed by using

*Flow sheet for recovery of fluoride using powder of spent cation-exchange resin loaded with zirconium(IV).*

adsorbents produced from various waste materials at cheap cost.

, the Japanese standard for fluoride, by add-

of tested sample solution. From these results, it

**8. Conclusion**

**140**

**Figure 26.**

The present work was conducted in part in the project of Water-Saving Recycling Systems in 2012–2013 supported by New Energy and Industrial Development Technology Organization (NEDO). The authors acknowledge the kind donation of sample of waste plating solution by Federation of Electro Plating Industry Association, Japan, and those of pulverized spent cation-exchange resin powder and orange juice residue by Muromachi Chemical Co. Ltd., Omuta, Japan, and JA Saga Beverage, Saga, Japan, respectively.

## **Author details**

Katsutoshi Inoue1 \*, Hari Paudyal1,2, Hidetaka Kawakita1,2 and Keisuke Ohto1

1 Department of Applied Chemistry, Faculty of Science and Engineering, Saga University, Saga, Japan

2 Central Department of Chemistry, Tribhuvan University, Kathmandu, Nepal

\*Address all correspondence to: kanoko1921@gmail.com

© 2018 The Author(s). Licensee IntechOpen. This chapter is distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/ by/3.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

## **References**

[1] Macaskill JB, Bates RG. Solubility product of calcium fluoride. The Journal of Physical Chemistry. 1977;**81**:496-498. DOI: 10.1021/j100520a026

[2] WHO. Guidelines for Drinking Water Quality, WHO, Geneva, Switzerland; 2004

[3] Helfferich F. Ion Exchange. McGraw-Hill; New York; 1962. pp. 250-323

[4] Yoshida I, Ueno K, Kobayashi H. Selective separation of arsenic (III) and (V) ions with ferric complex of chelating ion exchange resin. Separation Science and Technology. 1978;**13**:173- 184. DOI: 10.1080/01496397808057099

[5] Paudyal H, Pangeni B, Inoue K, Kawakita H, Ohto K, Harada H, Alam S. Adsorptive removal of fluoride from aqueous solution by using orange waste loaded with multivalent metal ions. Journal of Hazardous Materials. 2011;**192**:676-682. DOI: 10.1016/j. jhazmat.2011.05.070

[6] Paudyal H, Pangeni B, Inoue K, Matsueda M, Suzuki R, Kawakita H, Ohto K, Biswas BK, Alam S. Adsorption behavior of fluoride ions on zirconium(IV)-loaded orange waste gel from aqueous solution. Separation Science and Technology. 2012;**47**:96-103. DOI: 10.1080/01496395.2011.607204

[7] Paudyal H, Pangeni B, Inoue K, Kawakita H, Ohto K, Ghimire KN, Alam S. Preparation of novel alginate based anion exchanger from *Ulva japonica* and its application for the removal of trace concentrations of fluoride from water. Bioresource Technology. 2013;**148**:221-227. DOI: 10.1016/j.biortech.2013.08.116

[8] Paudyal H, Inoue K, Kawakita H, Ohto K, Kamata H, Alam S. Removal of fluoride by effectively using spent cation exchange resin. Journal of

Material Cycles and Waste Management. 2017;**20**:975-984. DOI: 10.1007/ s10163-017-0659-4

[9] Kraan S. Algal Polysaccharides. Novel Application and Outlook. Galway: Ocean Harvest Technology Ltd.; 2012. pp. 489-532

[10] Paudyal H, Pangeni B, Ghimire KN, Inoue K, Ohto K, Kawakita H, Alam S. Adsorption behavior of orange waste gel for some rare earth ions and its application to the removal of fluoride from water. Chemical Engineering Journal. 2012;**195-196**:289-296. DOI: 10.1016/j.cej.1012.04.061

[11] Paudyal H, Pangeni B, Inoue K, Kawakita H, Ohto K, Alam S. Removal of fluoride from aqueous solution by using porous resins containing hydrated oxide of cerium(IV) and zirconium(IV). Journal of Chemical Engineering of Japan. 2012;**45**:331-336. DOI: 10.1252/jcej.11we181

[12] Algagumuthu G, Rajan M. Equilibrium kinetics of adsorption of fluoride on to zirconium-impregnated cashew nut shell carbon. Chemical Engineering Journal. 2010;**158**:451-457. DOI: 10.1016/j.cej.2010.01.017

[13] Fang L, Ghimire KN, Kuriyama M, Inoue K, Makino K. Removal of fluoride using some lanthanum loaded adsorbents with different functional groups and polymer matrices. Journal of Chemical Technology and Biotechnology. 2003;**78**:1038-1047. DOI: 10.1002/jctb.902

[14] Meenakshi S, Viswanathan N. Identification of selective ion exchange resin for fluoride adsorption. Journal of Colloid and Interface Science. 2007;**308**:438-450. DOI: 10.1016/j. jcis.2006.12.032

[15] Zhou Y, Yu C, Shan Y. Adsorption of fluoride from aqueous solution on

**143**

*Adsorptive Removal of Fluoride onto Different Waste Materials: Orange Juice Residue, Waste…*

[23] Kemer B, Ozdes D, Gundogdu A, Bulut VN, Duran C, Soylak M. Removal of fluoride ions from aqueous solution by waste mud. Journal of Hazardous Materials. 2009;**168**:888-894. DOI: 10.1016/j.jhazmat.2009.02.109

[24] Wang SG, Ma Y, Shi YJ, Gong WX. Defluoridation performance and mechanism of nanoscale aluminum oxide hydroxide in aqueous solution. Journal of Chemical Technology and Biotechnology. 2009;**84**:1043-1050.

[25] Sundaram CS, Viswanathan N, Meenakshi S. Defluoridation of water using magnesia/chitosan composite. Journal of Hazardous Materials. 2009;**163**:618-624. DOI: 10.1016/j.

DOI: 10.1002/jctb.2131

jhazmat.2008.07.009

waters.2007.04.029

desal.2006.06.003

[26] Gupta VK, Ali I, Saini VK. Defluoridation of wastewaters using carbon slurry. Water Research. 2007;**41**:3307-3316. DOI: 10.1016/j.

[27] Tor A. Removal of fluoride from an aqueous solution by using montmorillonite. Desalination. 2006;**201**:267-276. DOI: 10.1016/j.

*DOI: http://dx.doi.org/10.5772/intechopen.80448*

La3+-impregnated cross-linked gelatin. Separation and Purification Technology.

[16] Yao R, Meng F, Zhang L, Ma D, Wang M. Defluoridation of water using neodymium-modified chitosan. Journal of Hazardous Materials. 2009;**165**:454- 460. DOI: 10.1016/j.jhazmat.2008.10.052

[17] Zhao Y, Li X, Liu L, Chen F. Fluoride

removal by Fe(III)-loaded ligand exchange cotton cellulose adsorbent from drinking water. Carbohydrate Polymers. 2008;**72**:144-150. DOI: 10.1016/j.carbpol.2007.07.038

[18] Viswananthan N, Sundaram CS, Meenakshi S. Removal of fluoride from aqueous solution using protonated chitosan beads. Journal of Hazardous Materials. 2009;**161**:423-430. DOI: 10.1016/j.jhazmat.2008.03.115

[19] Ku Y, Chiou HM. The adsorption of fluoride ion from aqueous solution by activated alumina. Water, Air, and Soil Pollution. 2002;**133**:349-361. DOI:

[20] Chikuma M, Nishimura M. Selective sorption of fluoride ions by anion exchange resin modified with alizarin fluorine blue-praseodymium complex. Reactive Polymers. 1990;**13**:131-138. DOI: 10.1016/0923-1137(90)90047-8

10.1023/A:101292990

[21] Puri BK, Balani S. Trace determination of fluoride using lanthanum hydroxide supported on alumina. Journal of Environmental Science and Health, Part A. 2000;**35**:109-121. DOI: 10.1080/10934.520009376957

[22] Mohan SV, Ramanaiah SV, Rajkumar B, Sharma PN. Biosorption of fluoride from aqueous solution onto algal *Spirogyra* IO1 and evaluation of adsorption kinetics. Bioresource Technology. 2007;**98**:1006-1011. DOI: 10.1016/j.biortech.2006.04.009

2004;**36**:89-94. DOI: 10.1016/ S1383-5866(03)00167-9

*Adsorptive Removal of Fluoride onto Different Waste Materials: Orange Juice Residue, Waste… DOI: http://dx.doi.org/10.5772/intechopen.80448*

La3+-impregnated cross-linked gelatin. Separation and Purification Technology. 2004;**36**:89-94. DOI: 10.1016/ S1383-5866(03)00167-9

[16] Yao R, Meng F, Zhang L, Ma D, Wang M. Defluoridation of water using neodymium-modified chitosan. Journal of Hazardous Materials. 2009;**165**:454- 460. DOI: 10.1016/j.jhazmat.2008.10.052

[17] Zhao Y, Li X, Liu L, Chen F. Fluoride removal by Fe(III)-loaded ligand exchange cotton cellulose adsorbent from drinking water. Carbohydrate Polymers. 2008;**72**:144-150. DOI: 10.1016/j.carbpol.2007.07.038

[18] Viswananthan N, Sundaram CS, Meenakshi S. Removal of fluoride from aqueous solution using protonated chitosan beads. Journal of Hazardous Materials. 2009;**161**:423-430. DOI: 10.1016/j.jhazmat.2008.03.115

[19] Ku Y, Chiou HM. The adsorption of fluoride ion from aqueous solution by activated alumina. Water, Air, and Soil Pollution. 2002;**133**:349-361. DOI: 10.1023/A:101292990

[20] Chikuma M, Nishimura M. Selective sorption of fluoride ions by anion exchange resin modified with alizarin fluorine blue-praseodymium complex. Reactive Polymers. 1990;**13**:131-138. DOI: 10.1016/0923-1137(90)90047-8

[21] Puri BK, Balani S. Trace determination of fluoride using lanthanum hydroxide supported on alumina. Journal of Environmental Science and Health, Part A. 2000;**35**:109-121. DOI: 10.1080/10934.520009376957

[22] Mohan SV, Ramanaiah SV, Rajkumar B, Sharma PN. Biosorption of fluoride from aqueous solution onto algal *Spirogyra* IO1 and evaluation of adsorption kinetics. Bioresource Technology. 2007;**98**:1006-1011. DOI: 10.1016/j.biortech.2006.04.009

[23] Kemer B, Ozdes D, Gundogdu A, Bulut VN, Duran C, Soylak M. Removal of fluoride ions from aqueous solution by waste mud. Journal of Hazardous Materials. 2009;**168**:888-894. DOI: 10.1016/j.jhazmat.2009.02.109

[24] Wang SG, Ma Y, Shi YJ, Gong WX. Defluoridation performance and mechanism of nanoscale aluminum oxide hydroxide in aqueous solution. Journal of Chemical Technology and Biotechnology. 2009;**84**:1043-1050. DOI: 10.1002/jctb.2131

[25] Sundaram CS, Viswanathan N, Meenakshi S. Defluoridation of water using magnesia/chitosan composite. Journal of Hazardous Materials. 2009;**163**:618-624. DOI: 10.1016/j. jhazmat.2008.07.009

[26] Gupta VK, Ali I, Saini VK. Defluoridation of wastewaters using carbon slurry. Water Research. 2007;**41**:3307-3316. DOI: 10.1016/j. waters.2007.04.029

[27] Tor A. Removal of fluoride from an aqueous solution by using montmorillonite. Desalination. 2006;**201**:267-276. DOI: 10.1016/j. desal.2006.06.003

**142**

*Environmental Chemistry and Recent Pollution Control Approaches*

Material Cycles and Waste Management.

[9] Kraan S. Algal Polysaccharides. Novel Application and Outlook. Galway: Ocean Harvest Technology Ltd.; 2012.

[10] Paudyal H, Pangeni B, Ghimire KN, Inoue K, Ohto K, Kawakita H, Alam S. Adsorption behavior of orange waste gel for some rare earth ions and its application to the removal of fluoride from water. Chemical Engineering Journal. 2012;**195-196**:289-296. DOI:

2017;**20**:975-984. DOI: 10.1007/

s10163-017-0659-4

10.1016/j.cej.1012.04.061

DOI: 10.1252/jcej.11we181

[12] Algagumuthu G, Rajan M. Equilibrium kinetics of adsorption of fluoride on to zirconium-impregnated cashew nut shell carbon. Chemical Engineering Journal. 2010;**158**:451-457.

DOI: 10.1016/j.cej.2010.01.017

[13] Fang L, Ghimire KN, Kuriyama M, Inoue K, Makino K. Removal of fluoride using some lanthanum loaded adsorbents with different functional groups and polymer matrices. Journal of Chemical Technology and Biotechnology. 2003;**78**:1038-1047. DOI: 10.1002/jctb.902

[14] Meenakshi S, Viswanathan N. Identification of selective ion exchange resin for fluoride adsorption. Journal of Colloid and Interface Science. 2007;**308**:438-450. DOI: 10.1016/j.

[15] Zhou Y, Yu C, Shan Y. Adsorption of fluoride from aqueous solution on

jcis.2006.12.032

[11] Paudyal H, Pangeni B, Inoue K, Kawakita H, Ohto K, Alam S. Removal of fluoride from aqueous solution by using porous resins containing hydrated oxide of cerium(IV) and zirconium(IV). Journal of Chemical Engineering of Japan. 2012;**45**:331-336.

pp. 489-532

[1] Macaskill JB, Bates RG. Solubility product of calcium fluoride. The Journal of Physical Chemistry. 1977;**81**:496-498.

[2] WHO. Guidelines for Drinking Water Quality, WHO, Geneva, Switzerland;

[3] Helfferich F. Ion Exchange. McGraw-Hill; New York; 1962. pp. 250-323

[4] Yoshida I, Ueno K, Kobayashi H. Selective separation of arsenic (III) and (V) ions with ferric complex of chelating ion exchange resin. Separation Science and Technology. 1978;**13**:173- 184. DOI: 10.1080/01496397808057099

[5] Paudyal H, Pangeni B, Inoue K, Kawakita H, Ohto K, Harada H, Alam S. Adsorptive removal of fluoride from aqueous solution by using orange waste loaded with multivalent metal ions. Journal of Hazardous Materials. 2011;**192**:676-682. DOI: 10.1016/j.

[6] Paudyal H, Pangeni B, Inoue K, Matsueda M, Suzuki R, Kawakita H, Ohto K, Biswas BK, Alam S. Adsorption

zirconium(IV)-loaded orange waste gel from aqueous solution. Separation Science and Technology. 2012;**47**:96-103. DOI: 10.1080/01496395.2011.607204

[7] Paudyal H, Pangeni B, Inoue K, Kawakita H, Ohto K, Ghimire KN, Alam S. Preparation of novel alginate based anion exchanger from *Ulva japonica* and its application for the removal of trace concentrations of fluoride from water. Bioresource Technology. 2013;**148**:221-227. DOI: 10.1016/j.biortech.2013.08.116

[8] Paudyal H, Inoue K, Kawakita H, Ohto K, Kamata H, Alam S. Removal of fluoride by effectively using spent cation exchange resin. Journal of

behavior of fluoride ions on

jhazmat.2011.05.070

DOI: 10.1021/j100520a026

**References**

2004

**145**

**Chapter 8**

**Abstract**

**1. Introduction**

inside the cell [3, 4].

**2. Copper bioremediation**

Bioremediation of Heavy Metals

Exposure to lead (Pb), zinc (Zn), cadmium (Cd), copper (Cu), and selenite (SeO3−2) consider the main heavy metals that threat human health. These heavy metals can interfere with the function of vital cellular components. Soil heavy metal contamination represents risks to humans and the ecosystem through drinking of contaminated groundwater, direct ingestion or the food chain, and reduction in food quality. Bioremediation means cleanup of polluted environment via transformation of toxic heavy metals into less toxic form by microbes or its enzymes. Otherwise, bioremediation by microbes has limitations like production of toxic metabolites. The efflux of metal ions outside the cell, biosorption to the cell walls and entrapment in extracellular capsules, precipitation, and reduction of the heavy

metal ions to a less toxic state are mechanisms to metals' resistance.

**Keywords:** heavy metals, bioremediation, copper, lead, cadmium, selenite

Since the industrial revolution, heavy metals' waste has increased rapidly. Toxic metals' species are mobilized from industrial activities and fossil fuel consumption and eventually are accumulated through the food chain, leading to both ecological and health problems. Some of these metals are taken up as essential nutrients since they are incorporated into enzymes and cofactors. Some heavy metals exert toxic effects on microbial cells (i.e., mercury, lead, cadmium, arsenic, and silver). Mostly, resistance systems have been found on plasmids, whereas bacterial chromosomes contain genes for resistance to many of the same heavy metals' cations and oxyanions as do plasmids [1, 2]. To survive under metal-stressed conditions, bacteria have evolved several types of mechanisms to tolerate the uptake of heavy metal ions. These mechanisms include biosorption to the cell walls and entrapment in extracellular capsules, precipitation, the efflux of metal ions outside the cell, reduction of heavy metal ions to a less toxic state accumulation, and complexation of metal ions

In almost all life forms, copper is a metal essential for the normal function. It acts as a cofactor for a number of enzymes involved in respiration and electron transport proteins in plants, animals, and microorganisms. Copper is toxic to cells at high concentrations mainly due to the disruption of the integrity of cell membranes, its interaction with nucleic acids, interference with the energy transport system, and disruption of enzyme active sites [5–8] . At high cytoplasmic

*Medhat Rehan and Abdullah S. Alsohim*

## **Chapter 8**
